NITRIC OXIDE-RELEASING POLYURETHANE MEMBRANES FOR IMPLANTABLE ELECTROCHEMICAL GLUCOSE SENSORS
A dissertation submitted to the faculty of the University of North Carolina at Chapel Hill in the partial fulfillment of the requirements for the degree of Doctor of Philosophy in the
Department of Chemistry (Analytical Chemistry).
Chapel Hill 2013
©2013 Ahyeon Koh
AHYEON KOH: Nitric Oxide-Releasing Polyurethane Membranes For Implantable Electrochemical Glucose Sensors
(Under the direction of Professor Mark H. Schoenfisch)
The development of novel biocompatible membranes is key to mitigating the host foreign body response (FBR) that limits the utility of implantable electrochemical biosensors for continuous glucose monitoring. Nitric oxide (NO)—an endogenously produced physiological mediator involved in wound healing, angiogenesis, and the inflammatory response—has been shown to reduce the FBR and may enhance sensor utility when released from sensor membranes.
Nitric oxide-releasing glucose sensor membranes with tunable release kinetics and total payloads were fabricated utilizing polyurethane (PU) films doped with NO donor-modified silica nanoparticles. A wide range of NO-release fluxes (5−460 pmol cm -2 s-1) and durations (16 h to 14 d) were achieved by altering the type of dopant, as well as
the PU sensor membrane composition and concentration. Sensor performance was affected by water uptake and membrane thickness regardless of the type of NO-release vehicle.
electrospinning. Electrospun PU fibers doped with NO-releasing silica particles exhibited a wide range of NO-release totals and durations (7.5−120 nmol mg-1 and 7 h to 14 d, respectively). These materials exhibited ~83% porosity with flexible plastic or elastomeric behavior, and a wide range of fiber diameters (119−614 nm) and mechanical strength (moduli of 1.7−34.5 MPa).
Nitric oxide-releasing electrospun fibers were applied to needle-type glucose sensors as the outermost membrane. The NO-releasing dendrimer-doped PU fiber mats maintained their porosity in serum without dendrimer leaching. Sensor performance was not significantly impacted by the additional porous membrane (≤50 µm thickness). The glucose sensitivity was 2.4 ± 1.6 nA/mM with a dynamic range 1–24 mM, indicating clinically acceptable performance.
My dissertation work would not be possible without support. Foremost, I do appreciate my advisor, Dr. Mark H. Schoenfisch, for all of his mentoring, patience, and support. He has fostered me as an independent scientist and has driven me to achieve the highest quality of research by providing a collaborative scientific environment.
I am grateful for all the support of past and present members in the Schoenfisch lab and other collaborators. The work presented herein could not have been completed without the assistance of Dr. Daniel Riccio, Dr. Bin Sun, Dr. Alexis Carpenter, and Dr. Yuan Lu who provided NO-releasing materials and shared their knowledge. I greatly thank Dr. Scott Nichols, Danielle Slomberg, Rebecca Hunter, Dr. Peter Coneski, Nga Brown, and Dr. Bruce Klitzman for helping me to conduct experiments and providing great insights on my projects. I also thank Wesley Storm, Katey Reighard, Chris Backlund, Justin Johnson, Brittany Worley, Angela Broadnax, and Robert Soto for providing great discussions, motivation, and friendships. During my time at UNC, I was fortunate to work with the most creative and intelligent scientists as well as to call all of them my friends.
TABLE OF CONTENTS
LIST OF TABLES ... xi
LIST OF FIGURES ... xiii
LIST OF ABBREVIATIONS AND SYMBOLS ... xviii
CHAPTER 1. BIOCOMPATIBLE MEMBRANES FOR IMPLANTABLE ELECTROCHEMICAL GLUCOSE SENSORS ...1
1.1 Electrochemical continuous glucose monitoring biosensors ...1
1.1.1 Overview of implantable electrochemical glucose sensors ...1
1.1.2 Implantable glucose sensor design and challenges for bioanalytical performance ...8
1.2 Biocompatibility concerns for subcutaneously implanted glucose sensors ...10
1.2.1 The effect of the foreign body response on in vivo glucose sensor performance ...11
1.3 Current strategies to improve biocompatibility of sensor membranes ...15
1.3.1 Active release ...16
1.3.2 Nitric oxide-releasing membranes ...19
1.3.3 Passive coatings ...26
1.3.4 Electrospinning porous membrane ...30
1.4 Summary of dissertation research ...33
CHAPTER 2. FABRICATION OF NITRIC OXIDE-RELEASING
POLYURETHANE GLUCOSE SENSOR MEMBRANES ...57
2.1 Introduction ...57
2.2 Material and methods ...60
2.2.1 Reagents and Materials ...60
2.2.2 Preparation of NO-releasing dopant ...61
2.2.3 Hybrid sol-gel/polyurethane glucose sensor fabrication ...61
2.2.4 Film fabrication and methods of film study ...63
2.2.5 Sensor performance of hybrid sol-gel/polyurethane glucose sensor ...65
2.3 Results and Discussion ...66
2.3.1 NO-releasing glucose sensor ...66
2.3.2. Variation of type of NO donors ...68
2.3.3 Variation of an additional polyurethane layer to alter NO release kinetics ...75
2.3.4. Variation of amount of silica particles doped within polyurethane film ...81
2.4 Conclusion ...84
2.5 References ...86
CHAPTER 3. NITRIC OXIDE-RELEASING SILICA NANOPARTICLE-DOPED POLYURETHANE ELECTROSPUN FIBERS ...91
3.1 Introduction ...91
3.2 Experimental ...94
3.2.1 Materials ...94
3.2.3 Nitric oxide-releasing silica particle-doped polyurethane
fiber formation. ...96
3.2.4 Characterization of NO-releasing silica particle-doped electrospun fibers ...97
3.3 Results and Discussion ...99
3.3.1 Fabrication of NO-releasing silica particle-doped electrospun fiber mats ...99
3.3.2 Nitric oxide release from silica nanoparticle-doped electrospun fiber mat ...113
3.4 Conclusion ...123
3.5 References ...124
CHAPTER 4. FABRICATION OF NITRIC OXIDE-RELEASING POROUS POLYURETHANE MEMBRANES COATED NEEDLE-TYPE IMPLANTABLE GLUCOSE BIOSENSORS ...131
4.1 Introduction ...131
4.2 Experimental ...133
4.2.1 Materials ...133
4.2.2 Fabrication of needle-type glucose sensors ...134
4.2.3 Nitric oxide-releasing dendrimer-doped polyurethane solution. ...137
4.2.4 Electrospinning of the outermost glucose sensor membrane ...139
4.2.5 Characterization of NO-releasing dendrimer-doped electrospun fiber membrane. ...139
4.2.6 Cytotoxicity assay. ...142
4.2.7 Electrochemical sensor performance ...143
4.3.1 Characterization of NO-releasing dendrimer-doped
electrospun polyurethane fibers ...144
4.3.2 Electrochemical performance of electrospun membrane coated glucose biosensor ...153
4.4 Conclusion ...157
4.5 References ...158
CHAPTER 5. IN VIVO PERFORMANCE OF PERCUTANEOUSLY IMPLANTED NITRIC OXIDE-RELEASING GLUCOSE SENSORS IN A FREELY MOVING PORCINE MODEL ...163
5.1 Introduction ...163
5.2 Methods and materials ...166
5.2.1 Materials ...166
5.2.2 Fabrication of NO-releasing needle-type glucose microsensors ...167
5.2.3 Characterization of NO-releasing glucose sensors ...170
5.2.4 Implantation and in vivo evaluation of sensor performance ...170
5.2.5 Data analysis for sensor accuracy in vivo ...172
5.3 Results and discussion ...174
5.3.1 In vitro electrochemical glucose sensor performance and nitric oxide release properties ...174
5.3.2 In vivo glucose sensor performance ...179
5.4 Conclusions ...187
5.5 References ...188
CHAPTER 6. SUMMARY AND FUTURE DIRECTIONS ...192
6.2 Future Directions ...195 6.2.1 Topography controlled co-axial electrospun fibers ...195 6.2.2 The topographical effect of localized NO delivery on the
foreign body response ...199 6.2.3 Percutaneous implantation of nitric oxide-releasing porous
membrane coated sensors for real-time glucose monitoring
in healthy and diabetic porcine model ...200 6.3 References ...202
LIST OF TABLES
Table 2.1. Characterization of NO-releasing silica particles ...62 Table 2.2. Characterization of NO release from NO donor-doped polyurethane
membranes. ...71 Table 2.3. Analytical performance criteria of glucose sensors with NO
donor-doped polyurethane membranes. ...73 Table 2.4. Characterization of NO release and glucose sensor performance for
NO-releasing AEAP3/TMOS particle-doped (0.6 mg·cm-2) polyurethane sensor membranes as a function of additional
top-casted polymer layer composition ...76 Table 2.5. Characterization of NO release and glucose sensor performances for
NO-releasing AEAP3/TMOS particle-doped (0.6 mg·cm-2) polyurethane sensor membrane as a function of additional TPU
polymer layer concentration ...80 Table 2.6. Characterization of NO release and glucose sensor performance for
S-nitrosothiol-modified MPTMS/TMOS particle-doped polyurethane
sensor membranes as a function of dopant concentration ...82 Table 3.1. Characterization of nitric oxide-releasing silica particles ...95 Table 3.2. Conductivity of initial polymer solution and resulting fiber diameter
as a function of dopant type. ...108 Table 3.3. Silica particle leaching from NO-releasing silica particle-doped
polyurethane electrospun fiber mats as a function of type of
polyurethane and dopant after 7 d soaking in PBS at 37 oC ...114 Table 3.4. Nitric oxide release characteristics of 5 wt% NO-releasing silica
particle-doped 12% (w/v) electrospun fiber mats ...116 Table 4.1. Nitric oxide-release properties of N-diazeniumdiolated
1,2-epoxy-9-decene functionalized poly(amidoamine) fourth generation dendrimers (PAMAM G4-ED/NO) in PBS (0.01 M, pH 7.4) at 37
oC. ...138 Table 4.2. Characterization of NO release and glucose sensor performance for
were doped with 5 wt% N-diazeniumdiolated dendrimers (PAMAM
G4-ED/NO). ...146 Table 5.1. Glucose sensitivity changes in various biological fluids ...176 Table 5.2. In vivo numerical and clinical accuracy of control and NO-releasing
sensors as a function of implantation period ...181 Table 5.3. Total number of data points and percent points in the zone of the
LIST OF FIGURES
Figure 1.1. The enzymatic oxidation of glucose to gluconolactone by glucose oxidase with subsequent electrochemical detection of oxygen
depletion and/or hydrogen peroxide formation ...4 Figure 1.2. Sensor design percutaneous (left) and fully implantable
subcutaneous (right) electrochemical glucose biosensors ...6 Figure 1.3. The foreign body response to a percutaneous glucose sensor upon
tissue implantation. Arrows in the magnified area show diffusion of glucose form blood vessels toward the sensor through native tissue (e.g., adipocytes), the collagen capsule, localized inflammatory cells, and biofouling layer near the sensor surface. As illustrated, glucose may be consumed by native tissue or inflammatory cells prior to
reaching the sensor ...12 Figure 1.4. (A) N-diazeniumdiolate and (B) S-nitrosothiol nitric oxide (NO)
donors with decomposition pathways. Decomposition kinetics is dependent on the chemical structure of the NO donor, pH,
temperature, and/or presence of other biological milieu ...22 Figure 2.1. Background current of particle-doped glucose sensor with
RSNO-modified particles (0.6 mg·cm-2) using applied potentials of (●) +0.80, (○) +0.65, and (■) +0.60 V vs. Ag/AgCl and with control (i.e., non-particle-doped) PU coated sensors (□) at +0.80 V vs.
Ag/AgCl ...67 Figure 2.2. Normalized glucose sensor sensitivity by sensitivity at 3 d for the
following sensors: (●) RSNO-MPTMS/TEOS particle-doped (0.6 mg·cm-2) glucose sensor; (○) non-NO-releasing particle-doped glucose sensor as a control; and (■) RSNO-MPTMS/TEOS particle-doped glucose sensor with an additional polyurethane layer (20
mg·mL-1 TPU) ...69 Figure 2.3. (A) Nitric oxide flux and (B) total NO release profile from
AEAP3/TMOS particle-doped polyurethane membranes as a function of additional PU layer composition (40 mg·mL-1): (●) Tecophilic HP-93A-100, (○) Hydrothane AL-25-80A, (■) Tecoflex
Figure 2.4. (A) Nitric oxide flux, and (B) NO totals from AEAP3/TMOS particle-doped (0.6 mg·cm-2) PU films (●) without and with additional Tecoflex SG-80A (TPU) layer at (○) 20, (■) 40, and (□)
60 mg·mL-1 concentration. ...79 Figure 2.5. (A) Nitric oxide flux and (B) total NO released from
RSNO-modified MPTMS/TEOS particle-doped polyurethane films as a function of particle concentration: (●) 0.2, (○) 0.6, (■) 1.2, and (□) 2.4 mg·cm-2. Inset of (A) provides enlarged view of NO flux after 7
d ...83 Figure 3.1. Environmental scanning electron microscopy images of 12% (w/v)
Tecoflex electrospun fibers doped with 5 wt% of N-diazeniumdiolated (A) AHAP3/TEOS (~50 nm), (B) AHAP3/TEOS (~100 nm), and (C) AEAP3/TMOS and (D) S-nitrosothiol
functionalized MPTMS/TEOS silica nanoparticles. ...102 Figure 3.2. Environmental scanning electron microscope images of polyurethane
electrospun fibers composed of 5 wt% N-diazeniumdiolated-AEAP3/TMOS nanoparticle-doped 8% (w/v) (A) Tecophilic, (B) Tecoflex, and (C) Tecoplast; and 12% (w/v) (D) Tecophilic, (E)
Tecoflex, and (F) Tecoplast PU polymer. Scale bar indicates 1 µm. ...103 Figure 3.3. (A) Kinematic viscosity of polymer solution and (B) diameters of
resulting fibers from polyurethanes doped with 5 wt% N-diazeniumdiolated AEAP3/TMOS silica nanoparticles as a function
of polymer concentration and type. ...105 Figure 3.4. Diameters of 5 wt% particle-doped 12% (w/v) polyurethane
electrospun fibers as a function of polyurethane type and NO-releasing silica particle dopant. Data is presented as mean ± standard
deviation (n=3, >250 measurements). ...106 Figure 3.5. Environmental scanning electron microscopy images of 12% (w/v)
Tecoplast electrospun fiber mat (A) without and (B) with 5 wt% of
N-diazeniumdiolated AEAP3/TMOS particles. ...109 Figure 3.6. Tensile stress-strain curves of (A) 5 wt% AEAP3/TMOS
particle-doped 12% (w/v) electrospun fiber mats as a function of polyurethane type: Tecophilic (●), Tecoflex (○), and Tecoplast ( ), and (B) 12% (w/v) Tecophilic electrospun fiber mats as a control (●) and a function of 1 ( ), 5 (■), and 10 wt% ( ) AEAP3/TMOS
Figure 3.7. (A) Nitric oxide flux and (B) NO totals from 5 wt% AHAP3/TEOS (~50 nm) particle-doped electrospun polyurethane fiber mats with 12% (w/v) of (●) Tecophilic, (○) Tecoflex, and (■) Tecoplast
polyurethane. ...118 Figure 3.8. (A) Nitric oxide flux and (B) NO totals from 5 wt% AHAP3/TEOS
(~100 nm) particle-doped electrospun polyurethane fiber mats with 12% (w/v) (●) Tecophilic, (○) Tecoflex, and (■) Tecoplast
polyurethane. ...120 Figure 3.9. Environmental scanning electron microscopy images of
AEAP3/TMOS particle-doped 12% (w/v) Tecophilic electrospun fiber mats as a function of dopant concentration, (A) 1, (B) 5, and
(C) 10 wt%. Scale bar indicates 5 µm. ...121 Figure 3.10. (A) Nitric oxide flux and (B) NO release totals from NO
donor-modified AEAP3/TMOS particle-doped 12% (w/v) Tecophilic electrospun polyurethane fiber mats as a function of dopant
concentration: 1 (●), 5 (○), and 10 (■) wt%. ...122 Figure 4.1. Amperometric response of 5 wt% NO-releasing dendrimer-doped
16% (w/v) Tecoplast electrospun fiber-modified needle-type glucose sensors without (i) or with (ii) an inner-selective layer. Glucose and interferences (i.e., ascorbic acid, acetaminophen, and uric acid) were sequentially injected into these solutions at physiologically relevant
concentrations. ...136 Figure 4.2. Schematics of (A) the layer-by-layer structure of NO-releasing
porous electrospun fiber membrane coated needle-type glucose sensors with actual fabricated electrode shown on the right; and (B) electrospinning configuration for coating outermost porous
membrane onto needle-type glucose sensors. ...140 Figure 4.3. Environmental scanning electron microscope (ESEM) images of (A)
NO-releasing dendrimer-doped electrospun polyurethane membrane on needle-type glucose sensors and (B) the cross sectional view with (i) a sol-gel/glucose oxidase enzyme layer, (ii) a diffusion-limiting polyurethane layer, and (iii) an electrospun fiber porous membrane; (C) NO-releasing dendrimer-doped electrospun fibers and inset indicating distribution of fiber diameters (540 ± 139 nm); and (D) confocal image of a single fiber embedded with RITC-labeled
Figure 4.4. Nitric oxide flux and total NO release from 5 wt% PAMAM G4-ED/NO dendrimer-doped 16% (w/v) Tecoplast electrospun
polyurethane fiber membranes. ...148 Figure 4.5. Relative viability of L929 mouse fibroblasts to polyurethane
electrospun fibers without (blank) and with dopant: non-NO-releasing dendrimer (control) and NO-non-NO-releasing dendrimer (i.e.,
PAMAM G4-ED/NO) for 24 and 48 h. ...150 Figure 4.6. Environmental scanning electron microscope (ESEM) images of the
sensor surface without porous membrane (A) and with NO-releasing dendrimer-doped outermost electrospun fiber membrane (B)
incubated in porcine serum for 7 d. ...152 Figure 4.7. Amperometric response of needle-type glucose sensors coated with
NO-releasing dendrimer (PAMAM G4-ED/NO)-doped membranes at a fiber mat thickness of (i) 45 to (ii) 72 and (iii) 242 µm. The
glucose concentration was changed at 3 mM increments. ...154 Figure 4.8. (A) Amperometric response of a needle-type glucose sensor for (i)
control (i.e., without) and (ii) 5 wt% NO-releasing dendrimer-doped 16% (w/v) Tecoplast electrospun fiber-modified outermost membrane. Glucose, ascorbic acid (AA), acetaminophen (AP), and uric acid (UA) were sequentially injected at relevant in vivo concentrations. (B) Calibration curves of (i) control and (ii) porous electrospun fiber membrane-modified glucose sensors in pH 7.4
Figure 5.1. Schematic diagram of the layered structure of S-nitrosothiol-modified NO-releasing silica particle (MPTMS/TEOS)-doped polyurethane coated needle-type glucose sensors. The resulting
electrode is shown to the far right. ...168 Figure 5.2. (A) Calibration curves for the needle-type customized Pinnacle
sensor (○) and fabricated NO-releasing sensor (●) in pH 7.4 PBS at room temperature with applied potential +0.6 V vs. Ag/AgCl. (B) Amperometric response of NO-releasing sensors upon sequential addition of 1 and 3 mM glucose (Glu) and 100 µM ascorbic acid,
uric acid, and urea. ...175 Figure 5.3. Nitric oxide-release profile from 72 mg/mL MPTMS/TEOS
particle-doped 50% (w/w) TPU/HPU polyurethane membrane coated
needle-type glucose biosensors. Inset represents integrated total NO release. ...178 Figure 5.4. Clarke Error Grid analysis for (A) controls and (B) NO-releasing
sensors (n=2 pigs and n=3 sensors). Presented data were cumulative
results for one-week implantation. ...183 Figure 6.1. Environmental scanning electron microscopy (ESEM) images of (A–
C) aligned and (D–E) random fibers collected on the window type of metal collector. Tecophilic (A and D), Tecoflex (B and E), and Tecoplast (C and F) polyurethane were electrospun on this collector. Insert image of each ESEM image is the fast Fourier transforms of
LIST OF ABBREVIATIONS AND SYMBOLS
oC Degree(s) Celsius
± Statistical margin of error
> Greater than
< Less than
≥ Greater than or equal to
≤ Less than or equal to
$ US dollar
×g Times the force of gravity
α Confidence interval
σ Standard deviation
ρ Density of the electrospun fiber mats ρ0 Density of the bulk polymer
AA Ascorbic acid
Ag/AgCl Silver/silver chloride reference electrode
AHAP N-(6-Aminohexyl)aminopropyl trimethoxysilane AHAP3 N-(6-Aminohexyl)aminopropyltrimethoxysilane AL-25-80A Hydrothane polyurethane
Ar Argon gas
ATCC American Type Culture Collection
BG Blood glucose concentration
CAM Chick chorioallantoic membrane CGM Continuous glucose monitoring
cm2 Square centimeter(s)
DETA/NO 1-[N-(Aminoethyl)-N-(2-ammonioethyl)amino] diazen-1-ium-1,2-diolate
DLS Dynamic light scattering
DMEM Dulbecco's modified Eagle's medium
DNA Deoxyribonucleic acid
e.g. For example
ECM Extra cellular membrane
EDRF Endothelial-derived relaxation factor
eNOS Endothelial NOS
ESEM Environmental scanning electron microscope et al. And others
etc. And so forth
FBGC Foreign body giant cell FBR Foreign body response FBS Fetal bovine serum
G4 Fourth generation
G(t) Glucose concentration
GDH Glucose dehydrogenase
GOx Glucose oxidase
H&E Hematoxylin and eosin
H2O2 Hydrogen peroxide
HP-93A-100 Tecophilic polyurethane
HPU Hydrothane AL 25-80A
i.e. That is
I(t) Current reading
I0 Background current
ICP-OES Inductively coupled plasma-optical emission spectroscopy IF Interstitial fluid
IgG Immunoglobulin G
iNOS Inducible NOS
KCl Potassium chloride
LFD Large-field detector
LMW Low molecular weight
MAD Mean absolute difference
MAP3 3-Methylaminopropyltrimethoxysilane MARD Mean absolute relative difference
MCP-1 Monocyte chemoattractant protein-1 MedAD Median absolute difference
MedARD Median absolute relative difference
mmHg Millimeter of mercury
MPTMS 3-Mercaptopropyltrimethoxysilane MTMOS Methyltrimethoxysilane
MTS 3-(4,5-Dimethylthiazol-2-yl)-5-(3-carboxymethoxyphenyl)-2-(4-sulfophenyl)-2H-tetrazolium inner salt
N2 Nitrogen gas
N/A Not applicable
nNOS Neuronal NOS
NO Nitric oxide
[NO]max Maximum NO flux
NOA Chemiluminescence Nitric Oxide Analyzer NOS Nitric oxide synthase
ONOO- Peroxynitrite !!! Permeability
PBS Phosphate buffered saline, pH 7.4 PCL Poly(ε-caprolactone)
pH -Log of proton concentration PLGA Poly(lactic-co-glycolic acid) PLLA Poly(L-lactic acid)
PMS Phenazine methosulfate ppb Parts per billion
ppm Parts per million
PROLI/NO 1-[(2-Carboxylato)pyrrolidin-1-yl]]diazen-1-ium-1,2-diolate PRP Platelet rich plasma
PS Penicillin streptomycin
RITC Rhodamine isothiocyanate rpm Revolution per minute RSNO S-Nitrosothiol
t95% Response time
tmax Time to max nitric oxide flux TEOS Tetraethoxysilane
TMOS Tetramethoxysilane TP-470 Tecoplast polyurethane
TPU Tecoflex SG-80A
UA Uric acid
U.S. The United States of America
VEGF Vascular endothelial growth factor
CHAPTER 1: BIOCOMPATIBLE MEMBRANES FOR IMPLANTABLE ELECTROCHEMICAL GLUCOSE SENSORS
Text, tables, and figures are adapted and reprinted with permission from the corresponding journal. Original articles are two papers: (1) a review article co-authored with Scott P. Nichols and Mark H. Schoenfisch published in Journal of Diabetes and Science Technology in 2011, titled “Glucose sensor membranes for mitigating the foreign body response”, vol. 5 (5), pp 1052-1059; and (2) a review article co-authored with Scott P. Nichols, Wesley L. Storm, Jae Ho Shin, and Mark H. Schoenfisch published in Chemical Reviews in 2013, titled “Biocompatible materials for continuous glucose monitoring devices”, vol. 113 (4), pp 2528-2549.
1.1 Electrochemical continuous glucose monitoring biosensors
1.1.1 Overview of implantable electrochemical glucose sensors
Diabetes mellitus is a worldwide epidemic characterized by chronic hyperglycemia that results from either a deficiency in or tolerance to insulin.1 In the United States, 8.3% of the population currently suffers from diabetes, with that number projected to increase to 1 in 3 adults by 2050 if current trends continue.2 Consequently, diabetes is the seventh leading cause of death in the United States with an annual cost burden of $174 billion.2
represent more than 85% of global market for biosensors in medical diagnostics.3,4 The traditional glucose monitoring techniques are primarily based on the use of electrochemical amperometric glucose sensors. The most successful technologies for measuring glucose concentrations are based on enzyme-modified electrodes and electrochemical amperometric detection with a number of useful designs. In 1967, Updike and Hicks first developed a sensor that detects glucose by monitoring the consumption of oxygen using two oxygen electrodes (one covered with the enzyme and one for reference), comparing the differential current between these electrodes to correct for background variations in oxygen.5 Alternatively, hydrogen peroxide produced enzymatically by glucose oxidase can be quantified amperometrically to indirectly determine glucose concentration, as first demonstrated by Guilbault and Lubrano in 1973.6 Amperometric enzyme-based glucose sensors vary greatly in electrode design, electrode material, enzyme immobilization method, and polymeric membrane compositions. To date, the U.S. Food and Drug Administration (FDA) has approved more than 25 glucose monitors, with the majority employing test strips consisting of either glucose dehydrogenase (GDH) or glucose oxidase (GOx) immobilized on a screen printed electrode.4 The analysis is based on obtaining a small blood sample (<1 µL) through a finger prick that is subsequently introduced into the test strip via capillary action.4,7
hyper- or hypoglycemic conditions. Additionally, the sample collection (i.e., finger prick) method is inconvenient and can be painful for adolescents, resulting in poor patient compliance. Analytical methods that enable continuous monitoring of blood glucose have thus been sought.8 Continuous glucose monitoring (CGM) provides real-time information on trends (i.e., whether the glucose levels are increasing or decreasing), magnitude, duration, and frequency of blood glucose fluctuations during the day.8,9 Ideally, analytically functional CGM devices could be linked to an insulin delivery pump, creating an artificial pancreas.8,9
Enzyme-immobilized amperometric biosensors have been implanted fully subcutaneously for month to years or percutaneously for <1 month, and most often only 3–5 days. Subcutaneous glucose sensors generally consist of a disk-type sensor with a titanium housing and measure oxygen consumption (Figure 1.2 right). Gough et al. reported on a subcutaneous sensor design based on differential electrochemical detection of oxygen via a two-step chemical reaction catalyzed by glucose oxidase and catalase.14 Accurate glucose measurements were carried out for >1 year by taking into account the difference in oxygen reduction at a working electrode producing a glucose-modulated current and a reference electrode producing an oxygen-dependent current.14 Sensor (oxygen) response changes due to collagen encapsulation, variations in local microvascular perfusion, and limitations in oxygen availability were thus relative, reducing the demand of device calibrations. The subcutaneous nature of the sensors likely minimizes any micromotion effects that also elevate the foreign body response (FBR).15 Unfortunately, implantation and subsequent replacement of the sensors required surgery, with each instance followed by a long (~2–3 week) stabilization period. Faulty devices for whatever reason would be costly to remove and/or replace. The size of the sensor is also significantly larger than percutaneous CGM systems (~3 cm vs. 350 µm) due to power (i.e., battery) requirements to support long-term use.
limiting membrane. Though such sensors are characterized as having a shorter stabilization period (e.g., 2‒4 h) compared to subcutaneous glucose sensors, the device penetrates through an opening in the dermis with concomitant infection and dislodging risks. Additionally, frequent calibration (e.g., >2 times per day) using intermittent glucose monitoring (via finger pricks) is required due to erratic analytical performance. The percutaneous nature of the device creates additional forces on the sensor that can lead to even greater inflammation.15 In this regard, compliance regarding the use of such devices remains poor. Nevertheless, only percutaneous implantable electrochemical glucose sensors are currently FDA approved and commercially available among the various continuous glucose monitoring technologies.18
membranes also exclude surface-active macromolecules (i.e., proteins and platelets), protecting the electrode from biofouling.4
Since the electrochemical detection of hydrogen peroxide requires oxygen, a cofactor in the GOx enzymatic reaction, oxygen concentration and fluctuation in vivo should be accounted for sensor design. Oxygen concentration in interstitial fluid is approximately ten times lower than the concentration of glucose resulting in an “oxygen deficit” state. Low concentrations of oxygen lead to problems with the biosensor response to glucose (particularly sensor sensitivity and linearity) due to stoichiometric imbalance between the two cofactors.11,22 Moreover, subcutaneous oxygen tension for humans ranges from 40 (~5 kPa) to 130 mm Hg (~17kPa) with partial pressures affected by anesthetics and hypoxia at the implantation site.23 Sensor performance issues due to changing oxygen levels are exacerbated by the foreign body response (FBR) that results in local consumption of oxygen and glucose by inflammatory cells at the vicinity of the sensor. Additionally, oxygen diffusion to the sensor decays exponentially after sensor implantation due to changes in tissue permeability.14 To overcome oxygen deficiency, polymeric membranes such as polyurethane, Nafion, silicone elastomer, polycarbonate, and layer-by-layer assembled polyelectrolytes are utilized to reduce glucose diffusion. 24-28 Polyurethane in particular is widely used as an outermost membrane of implantable
In addition to the issue of electroacitve interference and oxygen deficit for sensor fabrication, patient variability and physiological fluctuation are equally important factors for CGM device utility. Since percutaneous sensors are implanted through the epidermis, dermis, and subcutaneous layers, the effects of tissue heterogeneity are relevant to the analytical performance of the sensor. Temporal and spatial glucose dynamics are both influenced by tissue composition, distribution, and thickness.30-32 Temperature fluctuations in subcutaneous tissue will also impact sensor performance by altering glucose oxidase activity.33 Additionally, external pressure (e.g., posture change) on the CGM sensor has also caused erratic analytical performance.34 Such behavior is attributed in part to blood occlusion due to pressures applied to the tissue adjacent to the sensor.15,35 Moreover, these performance limitations may be more pronounced in diabetic patients due to differences in physiology.36 Therefore, these fluctuations and their possible impact on interstitial fluid physiology demand careful attention when characterizing in vivo sensor performance.
1.2 Biocompatibility concerns for subcutaneously implanted glucose sensors
improve the performance of medical devices in vivo. In general, the term “biocompatible” can be defined as material properties that avoid any negative local and systemic effects, and elicit the most appropriate local tissue response adjacent to an the implant allowing for improved performance.38 Along with this idea, most long-term medical implants to date are considered biocompatible or inert once the FBR resolves and the device is encapsulated by a collagen layer.39 Although CGM devices have similar circumstances, the combination of the FBR, oxygen and glucose availability, and need for immediate and frequent calibration have significantly impeded their utility and implementation as effective devices for diabetes management.
In the very early process of implantation, a provisional matrix instantaneously forms on and around foreign objects along with blood/material interactions and protein adhesion.19,37 The initial protein adsorption and fibrin-predominant provisional matrix is closely linked to the overall FBR by providing structural, biochemical, and cellular components for the inflammatory response.37 The chemoattractance, cytokines, growth factors, and other bioactive agents from the provisional matrix modulate the phenotype of macrophages as well as proliferation and activation of other cells.37 With this regard, the provisional matrix may be considered as a naturally derived membrane releasing bioactive agents to control subsequent phases of inflammatory response.37 In this stage, the adhesion of biomolecules to the sensor membrane typically results in a >50% decrease in the sensor response to glucose, with the greatest reduction in response caused by biomolecules <15 kDa.40-43 Proteomic analysis using mass spectroscopy of biomolecules adhered on implanted sensors in a rodent model showed both inflammatory cells and fragments of larger proteins infiltrated the sensor membranes and caused diminished glucose diffusivity.43 This protein adsorption is a time dependent process and mostly consists of biomolecules related to inflammatory response, including serum albumin, IgG, immunoglobulin, and fibrinogen.43 While this loss of sensitivity is reversible, the extent of signal reduction is unpredictable and requires frequent in vivo sensor calibration.10,41
response is to phagocytose the foreign material. The process of macrophages digesting the implant may further impact in vivo sensor performance due to the local pH drop as low as 3.6, which may negatively affect GOx activity.44 In the acute inflammatory stage, the released concentrations and types of chemokines and cytokines control the extent and/or degree of acute inflammatory response and the subsequent development of the FBR based on cell recruitment and ultimate phagocytosis.45 Additionally, the activation state (i.e., M1 or M2) of the macrophage is an important factor that influences the overall FBR.46 While limited studies have demonstrated distinct surface-induced phenotypes of macrophages on the wound healing process, the phenotype of activated macrophages is considered an indicator of tissue response variable inflammatory mediators.46,47
precursor to fibrous capsule formation due to the persistence of macrophages and infiltration of fibroblasts to the wound site.40
During the final step in the immune sequence, a fibrous capsule is formed with collagen surrounding the implant to isolate it completely from the local tissue environment.37 The collagen encapsulation (typical thickness 50–200 µm) with absence of the microvasculature consequently prevents implant interaction with surrounding native tissue.52 As such, diffusion of glucose is inhibited and the sensor fails to measure/report the actual blood glucose level of host. Ultimately, thick fibrous encapsulation significantly increases the sensor lag time, while lower subcutaneous vessel density and diminished capsule porosity lead to attenuation of analyte (i.e., glucose and oxygen) diffusion and response.53-55
Overall, the complex immune reaction and all stages of the FBR should be considered when designing outer tissue contacting membranes for implantable sensors. The developments of biosensor membranes that may enhance tissue integration and mitigate the FBR are obviously important for reducing the deleterious effects of the FBR on glucose sensor performance.
1.3 Current strategies to improve biocompatibility of sensor membranes
roles on the FBR.37,38 Thus, the biocompatibility of the sensor membrane is the most important factor in mitigating the highly complex FBR and integrating a device into the surrounding tissue. This facilitates measurement of glucose with clinically relevant accuracy and short lag time over the lifetime of the in vivo biosensor.38 Current strategies for improving glucose sensor biocompatibility are grouped into two areas: active release and passive coatings. Active release relies on the release of pharmaceutical molecules that may modify the FBR and direct the wound healing process to favor tissue integration of the sensor. Alternatively, passive coatings rely on the modification of chemical or physical characteristics at the tissue-sensor interface.
1.3.1 Active release
In a recent initiative, implant coatings have been synthesized to release biologically active molecules or pharmaceutical agents to improve biocompatibility. Upon release from the coating to the surrounding tissue the molecules are intended to influence the immune response, reduce collagen encapsulation, and/or increase angiogenesis. Several parameters should be considered in the design of an active-releasing surface, including the desired active molecule, toxicity, release kinetics and duration, relative amount, and delivery with each parameter being dependent on the molecule’s properties.
analysis increased, indicating sensor accuracy was improved.61 While the histological analysis revealed increased vascularization in tissue up to 13 mm away from the pumps, Clarke Error Grid analysis indicated that only sensors 1 mm from the VEGF-eluting pumps showed sensor accuracy improvements versus controls.61,62 This study highlighted the importance of the spatial release profile of angiogenic drug to improve sensor performance in vivo. Although recent studies indicate the potential of VEGF to influence the vasculature adjacent to implanted materials, the corresponding increase in inflammation is particularly troublesome and would likely diminish glucose sensor performance.
DX must be delivered continuously (i.e., for the duration of an implant) in order to maintain any anti-inflammatory benefits. However, systemic use of DX can cause serious side effects by depressing the innate immune response, thus increasing the likelihood of infection.79,80
To fully circumvent the FBR, hydrogels that release both VEGF and DX from a membrane were studied to reduce the inflammatory response to the implant while increasing angiogenesis.57,59 Unfortunately, the DX release significantly diminished the angiogenic benefits of VEGF.57 Other reports have also shown that glucocorticoid steroids, and in particular DX, inhibit VEGF activity in vivo.81-83 While concurrent release would be a promising approach to address the FBR as a whole, two active release agents that affect the FBR in a synergistic or non-antagonistic manner have yet to be identified.
1.3.2 Nitric oxide-releasing membranes
Nitric oxide synthases exist as three isoforms: neuronal NOS (nNOS), endothelial NOS (eNOS), and inducible NOS (iNOS).88,89 The nNOS isoform is localized in neurons and skeletal muscles, and regulates synaptic signaling, muscle contractility and local blood flow.90 The eNOS isoform is exclusively present in the endothelium, and regulated blood pressure, platelet aggregation, leukocyte adherence, and vascular smooth muscle cell mitogenesis.91 Nitric oxide produced from the nNOS and eNOS isoforms is relatively low in concentration (i.e., nM). The iNOS isoform is expressed in a wide array of cells and tissues (e.g., macrophages and neutrophils), and becomes activated upon exposure to endogenous pro-inflammatory mediators and endotoxins such as lipopolysaccharide (LPS).92 Relatively high concentration (i.e., µM) of NO derived by iNOS involves wound repair and host defense in related to inflammation, infection, and diabetes.92
elevated NO concentrations, suggesting NO could reduce the localized inflammatory response at the device-tissue interface as well as mitigate the subsequent FBR.99 As such, NO may be able to accomplish the hypothesized actions of a dual DX/VEGF release while avoiding the antagonistic behavior between the drugs. Additionally, NO has a short half-life (<1 s in the presence of oxygen and hemoglobin) in biological milieu, arising from its high reactivity with transition metals, heme-containing proteins, and thiols.85,86 Thus, NO’s sphere of influence is limited to a few µm, thus eliminating undesirable cytotoxicity concerns.100,101 In the presence of superoxide (O2●-), NO will react to form peroxynitrite (ONOO-), an even greater oxidant involved in the inflammatory response.102 The demonstrated antibacterial activity of NO against both positive and gram-negative bacteria may also allow for a reduced risk of infection due to percutaneous implantation.103,104
Based on the potential of releasing membranes for reducing the FBR, NO-releasing glucose sensor membranes have been developed by the Schoenfisch lab.125,134,135 Since the harsh procedure required to modify membrane with N-diazeniumdiolate caused inadequate permeability of analyte, the NO-releasing glucose sensor membranes were fabricated by doping NO-releasing sol-gel particles in the polyurethane film125 or a hydrophilic polymer (i.e., poly(vinylpyrrolidone)) in NO-releasing xerogel film,135 as well as by micro-patterning NO-releasing xerogel membrane.134 Of note, these NO-releasing membranes exhibited adequate analyte diffusion, demonstrating compatibility of NO release with enzyme-based glucose sensing. Additionally, the fabricated NO-releasing glucose sensors demonstrated not only sufficient sensor performance but also reduced bacterial adhesion holding potential to prevent the risk of infection during percutaneous implantation.
that the mitigated FBR by NO release was thus at least partially responsible for the superior glucose recovery.136
Only one in vivo report evaluating the effect of NO release on subcutaneously implanted electrochemical glucose sensor performance has been published. Gifford et al. doped (Z)-1-[N-methyl-N-[6-(N-butylammoniohexyl)amino]]-diazen-1-ium-1,2-diolate (DBHD/NO) (i.e., LMW NO donor) into a polyurethane/polydimethylsiloxane glucose sensor membrane.100 These membranes released NO with average NO flux of 7.52 pmol·cm-2·s-1. All of the NO was released after only 18 h.100 Despite the quick depletion of NO, the analytical performance (i.e., sensor accuracy) of percutaneous NO-releasing sensors in rodent model was improved by 2.4 and 2.1% relative to controls on days 1 and 3, respectively. Histological analysis of the tissue adjacent to the sensors showed decreased inflammation at 24 but not 48 h.100 Additionally, the NO-releasing glucose sensor exhibited a ~30 min run-in time (i.e., time required to stabilize sensor response after implantation), whereas a 4–10 h run-in time was observed for control sensors.100 This work suggests that NO release may represent an important strategy for improving in vivo glucose sensor performance.
1.3.3 Passive coatings
circumvent the FBR, since certain materials may allow the implant to appear less foreign to the host. A wide range of biomolecules have been used to interact with the surrounding tissue and mitigate the FBR including collagen,140,141 chitosan,142 cellulose,143,144 heparin,145 and dextran.146,147 Although these materials are still capable of eliciting an immunogenic response and are often undesirably biodegradable,144,148 biomolecules may prove beneficial for in vivo use. For example, phospholipids—a major component of cell membranes—has utilized as an outer layer to disguise the implant as more native than foreign.149 These phospholipid membranes have a high resistance to biofouling, possibly arising from the high water uptake of the materials.150 However, the phospholipid membranes have exhibited poor stability when grafted onto medical devices.151 To improve stability, the phospholipids have been incorporated within polymers. The resulting phospholipid-containing polymers have shown favorable inflammatory response.152,153 Kim et al. reported that macrophage adhesion to the phospholipid-containing polymer was reduced at 3 d relative to controls; however, it was not significantly affected at 7, 14 and 21 d, indicating only short-term advantages in terms of reducing an inflammatory response.151 The general consensus is that despite the short-term benefits, phospholipid membranes are not capable of circumventing the FBR that plagues sensors.
exhibiting its potential as a material for glucose sensor fabrication and use.29 A number of studies have shown decreased collagen capsule formation and reduced FBGC adhesion by blending copolymers with PU (e.g., polyether PU, polycarbonate PU, and silicon modified PU).164-167 Biocompatibility aside, PU allows for sufficient oxygen transport while limiting glucose diffusion to the sensor.29 For these reasons, the outermost membranes of commercially available implantable glucose sensors mostly consist of PU.168
deposition while fostering vascularized cellular and tissue growth.184 Additionally, pore sizes of 30–40 µm may force macrophages into a reconstructive phenotype, but will not cause macrophages to spread or phagocytose the material.183,185
The mechanical properties of a material also impact the resulting host response when implanted. External forces exerted on an implanted device can elicit an additional inflammatory response in the surrounding tissue.15,186 Additionally, the modulus at the skin-device interface must be considered. The mismatches in the elastic modulus between an implant and the skin that surrounds the device (e.g., sensor) can result in sheer forces that induce a more severe FBR.187 For example, the modulus of small fiber materials (<6 µm) has proved critical, with lower modulus fibers (e.g., polyurethane) showing reduced capsule formation compared to higher modulus materials (e.g., polyethylene and polyester).188 This phenomenon poses a challenge in the design of percutaneous implanted glucose sensors because the modulii of the dermis and subcutaneous tissue fall in different ranges (56–260 and 0.12–23 kPa, respectively).15,189-191
1.3.4 Electrospinning porous membrane
favorably oriented ends of fiber surface, repelling until the dry fiber network arrives on the collector.178 Electrospun fiber mats have monodisperse fiber diameters and a open porous structure, which can be controlled by fabrication parameters, polymer solution properties, and manner of collection.180 The diameter, distribution, and shape of fibers are mostly affected by the viscosity and conductivity of the polymer solution. Additionally, solvent composition, electric field, distance between needle and collector, feed rate, and needle size can all affect the fiber properties.178,180,192,193 The various fiber assemblies (e.g., such as random or aligned fibers, patterned fibers, and even three-dimensional fibrous architectures) can be achieved by using dynamic collection devices (e.g., rotating drum and parallel gap electrodes).192 The resulting fiber mats exhibit high surface area to volume ratios, thus enabling cell infiltration and tissue incorporation due to the porous structure mimicking an extra cellular membrane (ECM).171,194 Additionally, electrospun fiber mats have superior mechanical properties and flexibilities in surface functionalization compared to their non-porous analogs.180,195 Moreover, therapeutic molecules such as antibiotics, DNA, growth factors, and anti-inflammatory drugs can be encapsulated and released in a controlled fashion.195 Indeed, the electrospun fibers have been widely studied for biomedical applications, including wound dressings, tissue engineering scaffolds, and drug carriers.194-197
(PLLA) nano-fibers had lower in vitro macrophage activation in the early inflammation stage (first 24 h) than micro-fibers, indicating the importance of fiber diameter (rater than fiber alignment) in determining the inflammatory response.201 In contrast, Cao et al. reported that both alignment and orientation of the electrospun fibers greatly modulates the FBR in vivo; collagen capsule thickness for poly(ε-caprolactone) (PCL) fibers was decreased when their orientation was either aligned (~5 fold reduction) or random (~9 fold reduction) compared to solid films made from the same polymer.171 The aligned fibers also demonstrated better cellular infiltration both in vivo and in vitro, while randomly oriented fibers exhibited distinct surface boundaries between the material and the fibrous capsule.171
Although electrospun fibers indicate great promise for use as biomaterials, only one report has been published for implantable glucose sensor applications. Wang et al. recently reported the randomly oriented polyurethane electrospun fibers coated on needle-type glucose sensors, utilizing the porous membrane as an outermost diffusion controlled membrane to mitigate the FBR.202 Due to the solvent-free process of electrospun fiber formation, porous electrospun fibers can be coated directly onto enzyme-based electrochemical biosensors without compromising glucose oxidase activity.202 However, the development of porous glucose sensor membranes incorporating an active release agent has not been reported to date.
where dexamethasone was incorporated into PLLA and PCL electrospun fibers exhibited distinct release durations (~1 month and 90 min, respectively) due to intermolecular interactions.203 Of note, only DX-releasing PLLA fibers (i.e., longer release duration) significantly reduced inflammatory capsule formation compared to control PLLA and PCL scaffolds and DX-releasing PCL fibers.203 This research highlighted that prolonged release of DX from porous materials may greatly benefit biomedical applications.
Coneski et al. reported on NO-releasing electrospun fibers.126 The LMW molecule (i.e., disodium 1-[2-(carboxylate)pyrrolidin-1-yl]diazen-1-ium-1,2-diolate (PROLI/NO)) was doped into polyurethane and poly(vinyl chloride) solutions, and electrospun onto grounded disk-type collector to achieve microsized polymer fibers. The NO-release kinetics were controlled by the hydrophobicity of polymer with a certain concentration of dopant. As expected, NO release was limited due to use of the LMW NO donor. Nevertheless, this work set the stage for future studies aimed at longer NO-releasing fibers and fabrication of biosensors with fibrous sensor membranes.
1.4 Summary of dissertation research
1) developing controllable NO-releasing silica particle-doped polyurethane film membranes (i.e., release kinetics and total payload) by using polymers with varied water uptake and tuning the concentration of NO donor;
2) developing NO-releasing silica particle-doped porous materials via electrospinning and characterizing the NO release, fiber diameter, and mechanical properties;
3) fabricating needle-type implantable glucose biosensors coated with NO-releasing dendrimer-doped porous electrospun polyurethane membranes to combine the most promising active and passive anti-FBR strategies;
4) evaluating in vivo performance of the NO-releasing silica particle-doped polyurethane film-coated glucose biosensors in a healthy porcine model to study the effect of NO.
(1) WHO “World Health Statistics 2012,” World Health Organization, 2012.
(2) “National diabetes fact sheet: national estimates and general information on diabetes and prediabetes,” U.S. Department of Health and Human Services, Centers for Disease Control and Prevention, Atlanta, GA, 2011.
(3) “Biosensors–A global market overview,” IndustryExperts, Hyderabad, India, 2012. BA326444671EN.
(4) Wang, J. "Electrochemical glucose biosensors" Chemical Reviews 2008, 108, 814-825.
(5) Updike, S. J.; Hicks, G. P. "The enzyme electrode" Nature 1967, 214, 986-988. (6) Guilbault, G. G.; Lubrano, G. J. "An enzyme electrode for the amperometric
determination of glucose" Analytica Chimica Acta 1973, 64, 439-455.
(7) Newman, J. D.; Turner, A. P. F. "Home blood glucose biosensors: a commercial perspective" Biosensors and Bioelectronics 2005, 20, 2435-2453.
(8) Heller, A. "Implanted electrochemical glucose sensors for the management of diabetes" Annual Review of Biomedical Engineering 1999, 1, 153-175.
(9) Wilson, G. S.; Hu, Y. B. "Enzyme based biosensors for in vivo measurements" Chemical Reviews 2000, 100, 2693-2704.
(10) Wilson, G. S.; Zhang, Y. "Introduction to the glucose sensing problem" In In Vivo Glucose Sensing; Cunningham, D. D., Stenken, J. A., Eds.; Wiley, 2010.
(11) Vaddiraju, S.; Burgess, D. J.; Tomazos, I.; Jain, F. C.; Papadimitrakopoulos, F. "Technologies for continuous glucose monitoring: Current problems and future promises" Journal of Diabetes Science and Technology 2010, 4, 1540-1562. (12) Degani, Y.; Heller, A. "Direct electrical communication between chemically
(13) Pishko, M. V.; Katakis, I.; Lindquist, S.-E.; Ye, L.; Gregg, B. A.; Heller, A. "Direct electrical communication between graphite electrodes and surface adsorbed glucose oxidase/redox polymer complexes" Angewandte Chemie International Edition in English 1990, 29, 82-84.
(14) Gough, D. A.; Kumosa, L. S.; Routh, T. L.; Lin, J. T.; Lucisano, J. Y. "Function of an implanted tissue glucose sensor for more than 1 year in animals" Science Translational Medicine 2010, 2, 42ra53.
(15) Helton, K. L.; Ratner, B. D.; Wisniewski, N. A. "Biomechanics of the sensor– tissue interface—Effects of motion, pressure, and design on sensor performance and the foreign body response—Part I: Theoretical framework" Journal of Diabetes Science and Technology 2011, 5, 632-646.
(16) Shichiri, M.; Asakawa, N.; Yamasaki, Y.; Kawamori, R.; Abe, H. "Telemetry glucose monitoring device with needle-type glucose sensor: A useful tool for blood glucose monitoring in diabetic individuals" Diabetes Care 1986, 9, 298-301. (17) Bindra, D. S.; Zhang, Y.; Wilson, G. S.; Sternberg, R.; Thevenot, D. R.; Moatti,
D.; Reach, G. "Design and in vitro studies of a needle-type glucose sensor for subcutaneous monitoring" Analytical Chemistry 1991, 63, 1692-1696.
(18) Henning, T. "Commercially available continuous glucose monitoring systems" In In Vivo Glucose Sensing; Cunningham, D. D., Stenken, J. A., Eds.; John Wiley & Sons, Inc., 2010.
(19) Wilson, G. S.; Gifford, R. "Biosensors for real-time in vivo measurements" Biosensors and Bioelectronics 2005, 20, 2388-2403.
(20) Barlett, P. N.; Cooper, J. M. "A review of the immobilization of enzymes in electropolymerized films" Journal of Electroanalytical Chemistry 1993, 362, 1-12. (21) Chen, X.; Matsumoto, N.; Hu, Y.; Wilson, G. S. "Electrochemically mediated
electrodeposition/electropolymerization to yield a glucose microbiosensor with improved characteristics" Analytical Chemistry 2002, 74, 368-372.
(23) Koschwanez, H. E.; Reichert, W. M. "In vitro, in vivo and post explantation testing of glucose-detecting biosensors: Current methods and recommendations" Biomaterials 2007, 28, 3687-3703.
(24) Cambiaso, A.; Delfino, L.; Grattarola, M.; Verreschi, G.; Ashworth, D.; Maines, A.; Vadgama, P. "Modelling and simulation of a diffusion limited glucose biosensor" Sensors and Actuators B: Chemical 1996, 33, 203-207.
(25) Galeska, I.; Chattopadhyay, D.; Moussy, F.; Papadimitrakopoulos, F. "Calcification-resistant nafion/Fe3+ assemblies for implantable biosensors" Biomacromolecules 2000, 1, 202-207.
(26) Ishihara, K.; Tanaka, S.; Furukawa, N.; Nakabayashi, N.; Kurita, K. "Improved blood compatibility of segmented polyurethanes by polymeric additives having phospholipid polar groups. I. Molecular design of polymeric additives and their functions" Journal of Biomedical Materials Research 1996, 32, 391-399.
(27) Tipnis, R.; Vaddiraju, S.; Jain, F.; Burgess, D. J.; Papadimitrakopoulos, F. "Layer by layer assembled semipermeable membrane for amperometric glucose sensors" Journal of Diabetes Science and Technology 2007, 1, 193-200.
(28) Moussy, F.; Harrison, D. J.; O'Brien, D. W.; Rajotte, R. V. "Performance of subcutaneously implanted needle-type glucose sensors employing a novel trilayer coating" Analytical Chemistry 1993, 65, 2072-2077.
(29) Zhang, Y.; Wilson, G. S. "In vitro and in vivo evaluation of oxygen effects on a glucose oxidase based implantable glucose sensor" Analytica Chimica Acta 1993, 281, 513-520.
(30) Groenendaal, W.; Basum, G. v.; Schmidt, K. A.; Hilbers, P. A. J.; vanRiel, N. A. W. "Quantifying the composition of human skin for glucose sensor development " Journal of Diabetes Science and Technology 2010, 4, 1032-1040.
(31) Alexeeva, N. V.; Arnold, M. A. "Impact of tissue heterogeneity on noninvasive near-infrared glucose measurements in interstitial fluid of rat skin" Journal of Diabetes Science and Technology 2010, 4, 1041–1054.
implications for needle length recommendations" Current Medical Research and Opinion2010, 26, 1519-1530.
(33) Myrer, J. W.; Gary Measom, R.; Durrant, E.; Fellingham, G. W. "Cold- and hot-pack contrast therapy: Subcutaneous and intramuscular temperature change"
Journal of Athletic Training1997, 32, 238-241.
(34) Gilligan, B. C.; Shults, M.; Rhodes, R. K.; Jacobs, P. G.; Brauker, J. H.; Pintar, T. J.; Updike, S. J. "Feasibility of continuous long-term glucose monitoring from a subcutaneous glucose sensor in humans" Diabetes Technology and Therapeutics 2004, 6, 378-386.
(35) Castle, J. R.; Ward, W. K. "Amperometric glucose sensors: Sources of error and potential benefit of redundancy" Journal of Diabetes Science and Technology 2010, 4, 221-225.
(36) Petrofsky, J. S. "The effect of type-2 diabetes-related vascular endothelial dysfunction on skin physiology and activities of daily living " Journal of Diabetes Science and Technology2011, 5, 657-667.
(37) Anderson, J. M.; Rodriguez, A.; Chang, D. T. "Foreign body reaction to biomaterials" Seminars in Immunology2008, 20, 86-100.
(38) Williams, D. F. "On the mechanisms of biocompatibility" Biomaterials 2008, 29, 2941-2953.
(39) Isenhath, S. N.; Fukano, Y.; Usui, M. L.; Underwood, R. A.; Irvin, C. A.; Marshall, A. J.; Hauch, K. D.; Ratner, B. D.; Fleckman, P.; Olerud, J. E. "A mouse model to evaluate the interface between skin and a percutaneous device"
Journal of Biomedical Materials Research Part A2007, 83, 915-22.
(40) Anderson, J. M. "Biological responses to materials" Annual Review of Materials Research2001, 31, 81-110.
(41) ThomeDuret, V.; Gangnerau, M. N.; Zhang, Y.; Wilson, G. S.; Reach, G. "Modification of the sensitivity of glucose sensor implanted into subcutaneous tissue" Diabetes & Metabolism1996, 22, 174-178.
"Influence of inflammatory cells and serum on the performance of implantable glucose sensors" Journal of Biomedical Materials Research 2001, 54, 69-75.
(43) Gifford, R.; Kehoe, J. J.; Barnes, S. L.; Kornilayev, B. A.; Alterman, M. A.; Wilson, G. S. "Protein interactions with subcutaneously implanted biosensors" Biomaterials 2006, 27, 2587-2598.
(44) Zhao, Q. H.; McNally, A. K.; Rubin, K. R.; Renier, M.; Wu, Y.; Rose-Caprara, V.; Anderson, J. M.; Hiltner, A.; Urbanski, P.; Stokes, K. "Human plasma α 2-macroglobulin promotes in vitro oxidative stress cracking of pellethane 2363-80A: In vivo and in vitro correlations" Journal of Biomedical Materials Research 1993, 27, 379-388.
(45) Luttikhuizen, D. T.; Harmsen, M. C.; VanLuyn., M. J. A. "Cellular and molecular dynamics in the foreign body reaction" Tissue Engineering 2006, 12, 1955-1970.
(46) Anderson, J. M.; Jones, J. A. "Phenotypic dichotomies in the foreign body reaction" Biomaterials 2007, 28, 5114-5120.
(47) Jones, J. A.; Chang, D. T.; Meyerson, H.; Colton, E.; Kwon, I. K.; Matsuda, T.; Anderson, J. M. "Proteomic analysis and quantification of cytokines and chemokines from biomaterial surface-adherent macrophages and foreign body giant cells" Journal of Biomedical Materials Research Part A 2007, 83A, 585-596.
(48) Zhao, Q.; Topham, N.; Anderson, J. M.; Hiltner, A.; Lodoen, G.; Payet, C. R. "Foreign-body giant cells and polyurethane biostability: In vivo correlation of cell adhesion and surface cracking" Journal of Biomedical Materials Research 1991, 25, 177-183.
(49) Anderson, J. M.; Defife, K.; McNally, A.; Collier, T.; Jenney, C. "Monocyte, macrophage and foreign body giant cell interactions with molecularly engineered surfaces" Journal of Materials Science: Materials in Medicine 1999, 10, 579-88.
(50) Kao, W. J.; Zhao, Q. H.; Hiltner, A.; Anderson, J. M. "Theoretical analysis of in vivo macrophage adhesion and foreign body gaint cell formation on polydimethylsiloxane, low density polyethylene, and polyetherurethanes" Journal of Biomedical Materials Research 1994, 28, 73-79.
phosphofructokinase in wounded rat skeletal muscle." American Journal of Physiology1989, 256, E788-E797.
(52) Sieminski, A. L.; Gooch, K. J. "Biomaterial-microvasculature interactions"
Biomaterials2000, 21, 2233-2241.
(53) Novak, M.; Yuan, F.; Reichert, W. "Modeling the relative impact of capsular tissue effects on implanted glucose sensor time lag and signal attenuation"
Analytical and Bioanalytical Chemistry2010, 398, 1695-1705.
(54) Sharkawy, A. A.; Klitzman, B.; Truskey, G. A.; Reichert, W. M. "Engineering the tissue which encapsulates subcutaneous implants. I. Diffusion properties" Journal of Biomedical Materials Research Part A1997, 37, 401-412.
(55) Jablecki, M.; Gough, D. A. "Simulations of the frequency response of implantable glucose sensors" Analytical Chemistry2000, 72, 1853-1859.
(56) Sung, J.; Barone, P. W.; Kong, H.; Strano, M. S. "Sequential delivery of dexamethasone and VEGF to control local tissue response for carbon nanotube fluorescence based micro-capillary implantable sensors" Biomaterials 2009, 30, 622-631.
(57) Norton, L. W.; Koschwanez, H. E.; Wisniewski, N. A.; Klitzman, B.; Reichert, W. M. "Vascular endothelial growth factor and dexamethasone release from nonfouling sensor coatings affect the foreign body response" Journal of Biomedical Materials Research Part A2007, 81, 858-869.
(58) Norton, L. W.; Tegnell, E.; Toporek, S. S.; Reichert, W. M. "In vitro characterization of vascular endothelial growth factor and dexamethasone releasing hydrogels for implantable probe coatings" Biomaterials2005, 26, 3285-3297.
(59) Patil, S. D.; Papadmitrakopoulos, F.; Burgess, D. J. "Concurrent delivery of dexamethasone and VEGF for localized inflammation control and angiogenesis"
Journal of Controlled Release2007, 117, 68-79.
(60) Klueh, U.; Dorsky, D. I.; Kreutzer, D. L. "Enhancement of implantable glucose sensor function in vivo using gene transfer-induced neovascularization"